- 462 Views
- Uploaded on

Download Presentation
## PowerPoint Slideshow about 'Fatigue Failure' - Faraday

Download Now**An Image/Link below is provided (as is) to download presentation**

Download Now

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Presentation Transcript

Fatigue failure is characterized by three stages

- Crack Initiation

- Crack Propagation

- Final Fracture

It has been recognized that a metal subjected to a repetitive or fluctuating stress will fail at a stress much lower than that required to cause failure on a single application of load. Failures occurring under conditions of dynamic loading are called fatigue failures.

MAE dept., SJSU

Fracture zone

Propagation zone, striation

Jack hammer component, shows no yielding before fracture.

MAE dept., SJSU

VW crank shaft – fatigue failure due to cyclic bending and torsional stresses

Propagation zone, striations

Crack initiation site

Fracture area

MAE dept., SJSU

Fracture surface of a failed bolt. The fracture surface exhibited beach marks, which is characteristic of a fatigue failure.

1.0-in. diameter steel pins from agricultural equipment.

Material; AISI/SAE 4140 low allow carbon steel

MAE dept., SJSU

This long term fatigue crack in a high quality component took a considerable time to nucleate from a machining mark between the spider arms on this highly stressed surface. However once initiated propagation was rapid and accelerating as shown in the increased spacing of the 'beach marks' on the surface caused by the advancing fatigue crack.

MAE dept., SJSU

Hawaii, Aloha Flight 243, a Boeing 737, an upper part of the plane's cabin area rips off in mid-flight. Metal fatigue was the cause of the failure.

MAE dept., SJSU

Fracture Surface Characteristics

Mode of fracture

Typical surface characteristics

Ductile

Cup and ConeDimplesDull SurfaceInclusion at the bottom of the dimple

Brittle Intergranular

ShinyGrain Boundary cracking

Brittle Transgranular

ShinyCleavage fracturesFlat

Fatigue

BeachmarksStriations (SEM)Initiation sitesPropagation zoneFinal fracture zone

MAE dept., SJSU

a =

- min

max =

Alternating stress

min

max

a =

2

min = 0

Mean stress

m =

a =

max / 2

min

max

+

m=

2

Fatigue Failure – Type of Fluctuating StressesMAE dept., SJSU

Typical testing apparatus, pure bending

Motor

Load

Rotating beam machine – applies fully reverse bending stress

Fatigue Failure, S-N CurveTest specimen geometry for R.R. Moore rotating beam machine. The surface is polished in the axial direction. A constant bending load is applied.

MAE dept., SJSU

The standard machine operates at an adjustable speed of 500 RPM to 10,000 RPM. At the nominal rate of 10,000 RPM, the R. R. Moore machine completes 600,000 cycles per hour, 14,400,000 cycles per day.

Bending moment capacity

20 in-lb to 200 in-lb

MAE dept., SJSU

Se

Infinite life

Finite life

S′e

= endurance limit of the specimen

Fatigue Failure, S-N CurveN > 103

N < 103

MAE dept., SJSU

′

′

Se =

Se =

Sut ≤ 200 ksi (1400 MPa)

0.5Sut

Sut> 200 ksi

100 ksi

Sut> 1400 MPa

700 MPa

Cast iron

Cast iron

0.4Sut

Sut< 60 ksi (400 MPa)

Sut ≥60 ksi

24 ksi

Sut< 400 MPa

160 MPa

Relationship Between Endurance Limit and Ultimate StrengthSteel

MAE dept., SJSU

′

Se =

Se =

Sut < 40 ksi (280 MPa)

Sut < 48 ksi (330 MPa)

0.4Sut

0.4Sut

Sut ≥ 40 ksi

Sut ≥ 48 ksi

14 ksi

19 ksi

Sut ≥ 330 MPa

Sut ≥ 280 MPa

130 MPa

100 MPa

Copper alloys

Copper alloys

For N = 5x108 cycle

Relationship Between Endurance Limit and Ultimate StrengthAluminum

Aluminum alloys

For N = 5x108 cycle

MAE dept., SJSU

Se

= endurance limit of the specimen (infinite life > 106)

Se

= endurance limit of the actual component (infinite life > 106)

Sf

= fatigue strength of the actual component (infinite life > 5x108)

S

Se

′

Sf

= fatigue strength of the specimen (infinite life > 5x108)

N

106

103

For materials that do not exhibit a knee in the S-N curve, the infinite life taken at 5x108 cycles

S

Sf

N

5x108

103

Correction Factors for Specimen’s Endurance LimitFor materials exhibiting a knee in the S-N curve at 106 cycles

MAE dept., SJSU

′

Se = Cload Csize Csurf Ctemp Crel (Se)

Sf = Cload Csize Csurf Ctemp Crel (Sf)

Pure bending

Cload = 1

Pure axial

Cload = 0.7

Pure torsion

Cload = 1 if von Mises stress is used, use 0.577 if von Mises stress is NOT used.

Combined loading

Cload = 1

Correction Factors for Specimen’s Endurance Limitor

- Load factor, Cload (page 326, Norton’s 3rd ed.)

MAE dept., SJSU

For rotating solid round cross section

d ≤ 0.3 in. (8 mm)

Csize = 1

0.3 in. < d ≤ 10 in.

Csize = .869(d)-0.097

8 mm < d ≤ 250 mm

Csize = 1.189(d)-0.097

Correction Factors for Specimen’s Endurance Limit- Size factor, Csize(p. 327, Norton’s 3rd ed.)

Larger parts fail at lower stresses than smaller parts. This is mainly due to the higher probability of flaws being present in larger components.

If the component is larger than 10 in., use Csize = .6

MAE dept., SJSU

d

d95 = .95d

dequiv = (

)1/2

0.0766

Rectangular parts

Solid or hollow non-rotating parts

dequiv = .37d

dequiv = .808 (bh)1/2

Correction Factors for Specimen’s Endurance LimitFor non rotating components, use the 95% area approach to calculate the equivalent diameter. Then use this equivalent diameter in the previous equations to calculate the size factor.

A95 = (π/4)[d2 – (.95d)2] = .0766 d2

MAE dept., SJSU

Correction Factors for Specimen’s Endurance Limit

- surface factor, Csurf(p. 328-9, Norton’s 3rd ed.)

The rotating beam test specimen has a polished surface. Most components do not have a polished surface. Scratches and imperfections on the surface act like a stress raisers and reduce the fatigue life of a part. Use either the graph or the equation with the table shown below.

MAE dept., SJSU

Correction Factors for Specimen’s Endurance Limit

- Temperature factor, Ctemp(p.331, Norton’s 3rd ed.)

High temperatures reduce the fatigue life of a component. For accurate results, use an environmental chamber and obtain the endurance limit experimentally at the desired temperature.

For operating temperature below 450 oC (840 oF) the temperature factor should be taken as one.

Ctemp = 1 for

T ≤ 450 oC (840 oF)

MAE dept., SJSU

Correction Factors for Specimen’s Endurance Limit

- Reliability factor, Crel(p. 331, Norton’s 3rd ed.)

The reliability correction factor accounts for the scatter and uncertainty of material properties (endurance limit).

MAE dept., SJSU

Fatigue stress concentration factor

Kf=1+ (Kt–1)q

(p. 340, Norton’s 3rd ed.)

Steel

Fatigue Stress Concentration Factor, KfExperimental data shows that the actual stress concentration factor is not as high as indicated by the theoretical value, Kt. The stress concentration factor seems to be sensitive to the notch radius and the ultimate strength of the material.

MAE dept., SJSU

Use the design equation to calculate the size

Se

Kf a =

n

Design process – Fully Reversed Loading for Infinite Life- Determine the maximum alternating applied stress (a )in terms of the size and cross sectional profile

- Select material → Sy, Sut

- Choose a safety factor → n

- Determine all modifying factors and calculate the endurance limit of the component → Se

- Determine the fatigue stress concentration factor, Kf

- Investigate different cross sections (profiles), optimize for size or weight

- You may also assume a profile and size, calculate the alternating stress and determine the safety factor. Iterate until you obtain the desired safety factor

MAE dept., SJSU

Sn = a (N)b equation of the fatigue line

A

A

S

S

B

B

Sf

Se

Sn = .9Sut

N

N

106

5x108

103

103

Point A

N = 103

Sn = .9Sut

Sn = Se

Sn = Sf

Point A

Point B

Point B

N = 103

N = 106

N = 5x108

Design for Finite LifeMAE dept., SJSU

logSe = loga + blog106

(.9Sut)2

Se

.9Sut

(

)

a

1

=

b

log

.9Sut

=

Se

log

⅓

Se

3

N

(

)

Se

Sn

=

106

Sn

Kf a =

n

CalculateSnand replace Sein the design equation

Design equation

Design for Finite LifeSn = a (N)b

log Sn = log a + b log N

Apply boundary conditions for point A and B to find the two constants “a” and “b”

MAE dept., SJSU

Gerber curve

Se

Alternating stress

Goodman line

m

Sut

Sy

Soderberg line

Mean stress

The Effect of Mean Stress on Fatigue LifeMean stress exist if the loading is of a repeating or fluctuating type.

Mean stress is not zero

MAE dept., SJSU

a

C

Safe zone

Alternating stress

m

The Effect of Mean Stress on Fatigue Life Modified Goodman DiagramSy

Se

Goodman line

Sut

Sy

Mean stress

MAE dept., SJSU

Goodman line

- Syc

Sut

The Effect of Mean Stress on Fatigue Life Modified Goodman Diagrama

Sy

Yield line

Se

C

Safe zone

+m

Sy

- m

MAE dept., SJSU

m≤0

Fatigue,

Fatigue,

Infinite life

Se

a

m

1

a=

Finite life

=

+

nf

nf

a

m

Se

Sut

1

=

+

Yield

Sy

Syc

Sn

Sut

a+ m=

a+ m=

Yield

ny

ny

The Effect of Mean Stress on Fatigue Life Modified Goodman Diagrama

Se

C

Safe zone

Safe zone

+m

Sy

Sut

- m

- Syc

MAE dept., SJSU

Calculate the stress concentration factor for the mean stress using the following equation,

Kfa

Sy

Kfm=

m

Fatigue design equation

Kf a

Kfmm

1

Infinite life

=

+

nf

Se

Sut

Applying Stress Concentration factor to Alternating and Mean Components of Stress- Determine the fatigue stress concentration factor, Kf, apply directly to the alternating stress → Kfa

- If Kf max < Sy then there is no yielding at the notch, use Kfm =Kf and multiply the mean stress by Kfm → Kfmm

- If Kf max > Sy then there is local yielding at the notch, material at the notch is strain-hardened. The effect of stress concentration is reduced.

MAE dept., SJSU

Calculate the alternating and mean principal stresses,

1a, 2a=(xa /2)±(xa /2)2+(xya)2

1m, 2m=(xm /2)±(xm /2)2+(xym)2

Combined LoadingAll four components of stress exist,

xaalternating component of normal stress

xmmean component of normal stress

xyaalternating component of shear stress

xymmean component of shear stress

MAE dept., SJSU

m′ = (1m+ 2m - 1m2m)1/2

2

2

2

2

′a

′m

1

=

+

nf

Se

Sut

Fatigue design equation

Infinite life

Combined LoadingCalculate the alternating and mean von Mises stresses,

MAE dept., SJSU

R1= 2500, R2= 7500 lb.

The critical location is at the fillet,

MA= 2500 x 12 = 30,000 lb-in

32M

305577

Mc

a=

Calculate the alternating stress,

=

=

I

πd 3

d 3

Determine the stress concentration factor

D

r

= 1.5

= .1

Kt = 1.7

d

d

10,000 lb.

Design Example6˝

6˝

12˝

A rotating shaft is carrying 10,000 lb force as shown. The shaft is made of steel with Sut = 120 ksi and Sy = 90 ksi. The shaft is rotating at 1150 rpm and has a machine finish surface. Determine the diameter, d, for 75 minutes life. Use safety factor of 1.6 and 50% reliability.

d

D = 1.5d

A

R1

R2

r (fillet radius) = .1d

m= 0

MAE dept., SJSU

Using r = .1and Sut = 120 ksi, q (notch sensitivity) = .85

Csurf = A (Sut)b = 2.7(120)-.265 = .759

0.3 in. < d ≤ 10 in.

Csize = .869(d)-0.097 = .869(1)-0.097 = .869

Design ExampleAssume d = 1.0 in

Kf= 1 + (Kt – 1)q = 1 + .85(1.7 – 1) = 1.6

Calculate the endurance limit

Cload = 1 (pure bending)

Crel = 1 (50% rel.)

Ctemp= 1 (room temp)

′

Se = Cload Csize Csurf Ctemp Crel (Se) = (.759)(.869)(.5x120) = 39.57 ksi

MAE dept., SJSU

(

)

log

⅓

.9x120

86250

(

)

Sn

39.57

=

= 56.5 ksi

106

Sn

56.5

305577

n =

a=

= .116 < 1.6

=

= 305.577 ksi

Kfa

1.6x305.577

d 3

So d = 1.0 in. is too small

Se

(

)

.9Sut

log

⅓

Assume d = 2.5 in

N

(

)

Se

Sn

=

All factors remain the same except the size factor and notch sensitivity.

106

Using r = .25and Sut = 120 ksi, q (notch sensitivity) = .9

Kf= 1 + (Kt – 1)q = 1 + .9(1.7 – 1) = 1.63

Se =36.2 ksi

→

Design ExampleDesign life, N = 1150 x 75 = 86250 cycles

Csize = .869(d)-0.097 = .869(2.5)-0.097 = .795

MAE dept., SJSU

(

)

log

⅓

.9x120

86250

(

)

Sn

36.20

=

= 53.35 ksi

305577

a=

106

= 19.55 ksi

(2.5)3

Sn

53.35

n =

= 1.67 ≈ 1.6

=

Kfa

1.63x19.55

d=2.5 in.

Check yielding

Sy

90

n=

2.8 > 1.6 okay

=

=

Kfmax

1.63x19.55

Design ExampleSe =36.2 ksi

→

MAE dept., SJSU

6˝

12˝

d

D = 1.5d

A

R1

R2 = 7500

Sn

r (fillet radius) = .1d

56.5

n =

Calculate an approximate diameter

= .116 < 1.6

=

Kfa

1.6x305.577

Sn

56.5

n =

→ d = 2.4 in.

=

= 1.6

So d = 1.0 in. is too small

Kfa

1.6x305.577/d 3

Check the location of maximum moment for possible failure

Design Example – ObservationsSo, your next guess should be between 2.25 to 2.5

Mmax (under the load) = 7500 x 6 = 45,000 lb-in

MA (at the fillet) = 2500 x 12 = 30,000 lb-in

But, applying the fatigue stress conc. Factor of 1.63,Kf MA = 1.63x30,000 = 48,900 > 45,000

MAE dept., SJSU

r

4

= .16

=

25

d

Kt = 1.76

D

35

=

= 1.4

d

25

ExampleA section of a component is shown. The material is steel with Sut = 620 MPa and a fully corrected endurance limit of Se = 180 MPa. The applied axial load varies from 2,000 to 10,000 N. Use modified Goodman diagram and find the safety factor at the fillet A, groove B and hole C. Which location is likely to fail first? Use Kfm = 1

Pm = (Pmax + Pmin) / 2 = 6000 N

Pa = (Pmax – Pmin) / 2 = 4000 N

MAE dept., SJSU

Calculate the alternating and the mean stresses,

Pa

4000

a=

1.65

= 52.8 MPa

Kf

=

A

25x5

Pm

6000

m=

= 48 MPa

=

A

25x5

Fatigue design equation

a

m

1

Infinite life

=

+

1

n

Sut

52.8

48

Se

n = 2.7

→

=

+

n

180

620

ExampleUsing r = 4and Sut = 620 MPa, q (notch sensitivity) = .85

Kf= 1 + (Kt – 1)q = 1 + .85(1.76 – 1) = 1.65

MAE dept., SJSU

Using r = 3and Sut = 620 MPa, q (notch sensitivity) = .83

Calculate the alternating and the mean stresses,

Pm

6000

m=

= 41.4 MPa

=

A

29x5

Pa

4000

a=

2.1

= 58.0 MPa

Kf

=

A

(35-6)5

1

58.0

41.4

n = 2.57

→

=

+

n

180

620

ExampleGroove

r

3

= .103

=

29

d

→ Kt= 2.33

D

35

=

= 1.2

d

29

Kf= 1 + (Kt – 1)q = 1 + .83(2.33 – 1) = 2.1

The part is likely to fail at the hole, has the lowest safety factor

MAE dept., SJSU

Fm= (Fmax + Fmin) / 2=22.5 lb.

Ma=7.5 x 16 = 120 in - lb

Mm=22.5 x 16 = 360 in - lb

32Ma

32(120)

Mc

a=

=

= 23178.6 psi

=

I

πd 3

π(.375)3

32Mm

32(360)

Mc

m=

= 69536 psi

=

=

I

πd 3

π(.375)3

ExampleThe figure shows a formed round wire cantilever spring subjected to a varying force F. The wire is made of steel with Sut = 150 ksi. The mounting detail is such that the stress concentration could be neglected. A visual inspection of the spring indicates that the surface finish corresponds closely to a hot-rolled finish. For a reliability of 99%, what number of load applications is likely to cause failure.

MAE dept., SJSU

A95= .010462d 2 (non-rotating round section)

dequiv= √ A95 / .0766 = .37d = .37 x.375 = .14

1

23178.6

69536

n = .7< 1

→

a

→

m

=

+

1

n

24077

150000

=

+

Finite life

n

Sut

Se

Find Sn, strength for finite number of cycle

a

m

23178.6

69536

Sn = 43207 psi

→

1

→

=

1

+

=

+

Sut

Sn

Sn

150000

ExampleCalculate the endurance limit

Csurf = A (Sut)b = 14.4(150)-.718 = .394

Cload = 1 (pure bending)

Ctemp= 1 (room temp)

Crel= .814 (99% reliability)

dequiv= .14 < .3 → Csize = 1.0

Se = Cload Csize Csurf Ctemp Crel (Se) = (.394)(.814)(.5x150) = 24.077 ksi

MAE dept., SJSU

Download Presentation

Connecting to Server..